IPST Technical Paper Series Number 849 Laccase-Mediator Systems and Oxygen Delignification-A Comparative Study F.S. Chakar, A.J. Ragauskas, and T.J. McDonough April 2000 Submitted to International Pulp Bleaching Conference Halifax, Nova Scotia, Canada June 27-30,2000 Copyright* 2000 by the Institute of Paper Science and Technology For Members On/y INSTITUTE OF PAPER SCIENCE AND TECHNOLOGY PURPOSE AND MISSIONS The Institute of Paper Science and Technology is an independent graduate school, research organization, and information center for science and technology mainly concerned with manufacture and uses of pulp, paper, paperboard, and other forest products and byproducts. Established in 1929 as the Institute of Paper Chemistry, the Institute provides research and information services to the wood, fiber, and allied industries in a unique partnership between education and business. The Institute is supported by 52 North American companies. The purpose of the Institute is fuifilled through four missions, which are: 0 to provide multidisciplinary graduate education to students who advance the science and technology of the industry and who rise into leadership positions within the industry; * to conduct and foster research that creates knowledge to satisfy the technological needs of the industry; to provide the information, expertise, and interactive learning that enables customers to improve job knowledge and business performance; 0 to aggressively seek out technological opportunities and facilitate the transfer and implementation of those technologies in collaboration with industry partners. ACCREDITATION The Institute of Paper Science and Technology is accredited by the Commission on Colleges of the Southern Association of Colleges and Schools to award the Master of Science and Doctor of Philosophy degrees. NOTICE AND DISCLAIMER The Institute of Paper Science and Technology (IPST) has provided a high standard of professionalservice and has put forth its best efforts within the time and funds available for this project. The information and conclusions are advisory and are intended only for internal use by any company who may receive this report. Each company must decide for itself the best approach to solving any problems it may have and how, or whether, this reported information should be considered in its approach. IPST does not recommend particular products, procedures, materials, or service. These are included only in the interest of completeness within a laboratory context and budgetary constraint. Actual products, materials, and services used may differ and are peculiar to the operations of each company. In no event shall IPST or its employees and agents have any obligation or liability for damages including, but not limited to, consequential damages arising out of or in connection with any company’s use of or inability to use the reported information. IPST provides no warranty or guaranty of results. The Institute of Paper Science and Technology assures equal opportunity to all qualified persons without regard to race, color, religion, sex, national origin, age, disability, marital status, or Vietnam era veterans status in the admission to, participation in, treatment of, or employment in the programs and activities which the Institute operates. LACCASE-MEDIATOR SYSTEMS AND OXYGEN DELIGNIFICATIONA COMPARATIVE STUDY 18.0 16.0 14.0 F.S. Chakar 4 12.0 1 8 8.0 (0 A.J. Ragauskas T.J. McDonough 10.0 Institute of Paper Science and Technology 500 lofi Street, NW Atlanta, GA 303 18 ABSTRACT A conventional SW kraft pulp with an initial kappa number of 73.4 was subjected to a series of treatments using laccasevioluric acid (LMSvA=L),oxygen, and a combination of both systems. The treated pulps were characterized for kappa, brightness, and viscosity. Based on the experimental conditions employed in this study, an L, LE, and LLE exhibited superior retention in pulp viscosity than an 0 or a double 0. The delignificationresponse obtained with an LLE and an OLE treatment was comparable to a 00 stage. Relative to the brownstock, the laccase treated pulps were significantly lower in brightness. However, an E stage subsequent to an L treatment alleviated this effect. Overall, the application of laccasemediator systems on high-kappa pulps may be a viable technology that can yield substantial delignification without detrimental ramifications on viscosity. INTRODUCTION The bleaching of kraft pulps is a pivotal operation in the production of high-value paper products. Over the last two decades, research activities in pulp and paper have largely focused on environmental issues. As these issues continue to be addressed, new opportunities are developing. There has been a renewed interest in pulping and bleaching yields research [ 1-71. Improvements in yields will have positive ramifications on wood utilization practices, as well as on operating and capital cost associated with the production of kraft pulps. One promising method for improving pulp yield consists of halting the haft cook at a relatively high kappa (> 40). The pulp is then treated with a single or double oxygen stage before it is bleached. Recently, we have begun exploring competing enzymatic systems, more specifically laccase-mediator systems (LMS), as potential cost-effective alternatives to oxygen delignification [8,9]. Several research groups [ 10-151 have established the high selectivity of LMS and the ability to achieve substantial levels of delignification (> 45% delignification) on low-lignin content SW and H W kraft pulps (kappa # < 30). Based on these fmdings, we hypothesized that an LMS could delignify high-lignin content krafi pulps. Our initial results  shown in Figure 1 supported this claim 6.0 4.0 2.0 0.0 1 2 4 %HBTMODWp 6 Figure 1. Effect of 1-hydroxybenzotriazole (EIBT) charge on delignification of a 97.5 kappa commercial SW h a f t pulp with constant laccase charge. Further LMS studies on a conventional SW haft pulp (kappa # 73.4) demonstrated that violuric acid (VA) was a superior mediator with respect to both 1-hydroxybenzotriazole (HBT) and N-acetyl-N-phenylhydroxylamine(NHAA) [ 161. These results are summarized in Figure 2. 75.07 74..i 65.0 2 60.0 P xB 55.0 50.0 45.0 Figure 2. Kappa number of pulps subjected to LMS followed by an alkaline extraction, using equal molar doses of NHAA, HBT and VA. This report summarizes our continued efforts in examining LMS systems on high-kappa kraft pulps. The objective of this study was to compare the delignificationresponse of an LMSVA, and a two stage LMSvAto an oxygen and a double oxygen treatment. In addition, the delignification response of sequence treatments with both systems was also investigated. MATERIALS AND METHODS Materials All materials were purchased from Aldrich Chemical Co., Milwaukee, WI, and used as received, except for NHAA. NHAA was synthesized in accordance with Oxley’s [ 171 method. Laccase from Trametes villosa, was donated by Novo Nordisk Biochem, Franklinton, NC. Furnish A conventional southern USA softwood kraft pulp (kappa # 73.8) was prepared from Pinus faedu chips at Potlatch Corp. facilities in Cloquet, MN. The chips were cooked to an H-factor of 573 using 18.5% active alkali. The pulp was thoroughly washed, screened, centrifuged, fluffed, and stored at 4OC prior to carrying out experiments. Methods Enzyme assay Laccase activity was measured by monitoring the rate of oxidation of syringaldazine. One unit of activity (U)was defined as the change in absorbance at 53Onm of 0.001 per minute per ml of enzyme solution, in a 100 mM potassium phosphate buffer (2.2 ml) and 0.216 mh4 syringaldazine in methanol (0.3 ml,pH 6.7). The procedure was carried out at 23OC. The activity of the laccase was 1.87 E + 06 U/ml of enzyme solution. Laccase-mediator delignificationprocedure A 300-ml capacity Parr reactor equipped with a stirrer, a pressure gauge, a heating mantle, and connected to a Pan 4842 temperature controller was charged with 10 g of 0.d. fibers. The pulp consistency was adjusted to 10% with distilled water. The slurry was then heated to 45OC and was maintained at this temperature throughout the incubation period. VA (4.4 mmol/ 10 g of 0.d. pulp) was then added to the heated slurry. Subsequent to mixing the sluny (approx. 5 minutes), the pH was adjusted to 4.5 with glacial acetic acid or saturated sodium bicarbonate solution. Laccase (93,500 U, or 0.05 ml of enzyme solution/ g of 0.d. fiber) was added, and the reactor was sealed and pressurized with oxygen to 145 psig. After a mixing period of 1 hour, the pulp was removed from the reactor and thoroughly washed with distilled water (12L per 10 g of 0.d. pulp). The treated and washed pulp was either followed by subsequent treatments (oxygen delignification or LMS) or simply subjected to an alkaline extraction stage (E). Alkaline extraction stage Alkaline extractions (E) were carried out for 1hour at 80°C, 10% consistency in 4mm thick heat-sealable Kapak pouches. All E treatments employed 2.5% charge (0.d. basis) of NaOH. Oxygen delignification Oxygen delignification was carried out in a 300-ml capacity Parr reactor. All treatments were conducted at 95 OC, 10 % consistency, for 1 hour. A charge of 2.5% NaOH (0.d. basis) was employed. Subsequent to a treatment, the pulp was thoroughly washed with distilled water. Hexenuronic acid content in brownstock The content of hexenuronic acids in the brownstock was indirectly measured in accordance with a modified procedure reported by Vuorinen et al. . In brief, a 1000-ml round bottom flask was charged with 25 g of pulp (0.d. basis). The pulp consistency was adjusted to 3% by adding distilled water. The pH was then lowered to 3 using concentrated sulfuric acid. The slurry was refluxed for three hours at 100OC. The change in kappa number before and after the treatment was then determined and served as indirect measurement of hexenuronic acids (see Table I). Clearly, the hexenuronic acid content of this pulp was negligible. TABLE I. CHANGES IN KAPPA # AFTER ACID Initial kappa 73.4 73.4 Replicate /# 1 2 Final kappa 71.5 71.9 % change 2.6 2.0 Pulp characterization The kappa, brightness, and viscosity before and after treatments were measured in accordance with TAPPI Test Methods T236 and UM246, T452, and T230, respectively [ 19221. Only the terminal viscosity of the treated pulps was measured. The initial viscosity of the starting material could not be determined using TAPPI Test Method T230 due to the highlignin content in the pulp. Kappa and viscosity measurements were duplicated. Each brightness value was based on the average of five readings. Experimental design A conventional SW haft pulp with an initial kappa of 73.8 was subjected to a series of L (L= LMSVA)and oxygen delignification treatments. The list of experiments is summarized in Table II. TABLE 11. SUMMARY OF TREATMENTS Treatment # I Description 1 L 2 3 4 5 6 7 8 LE LLE 0 00 OLE LO OLO RESULTS Based on our previous studies [9,16], we have demonstrated that an LMSNHAA, an LMSHBT,and an LMSVAcan yield substantial delignification when applied on high-kappa pulps. However, under the experimental conditions used in our studies, we noted that VA outperformed both NHAA and HBT [ 161. This study summarizes our continued research efforts in this field. A conventional SW haft pulp (kappa # 73.4) was subjected to LMSVA,oxygen, double oxygen, and a combination of LMS and oxygen treatments. The pulps were then characterized for viscosity, kappa, and brightness. Kappa The delignification results shown in Figure 2 clearly demonstrate than an LMS system can yield substantial delignification on a high-kappa pulp. As expected, the delignificationeffect was further enhanced after an E stage, as the NaOH solubilizes the oxidized lignin. The data also suggest that under the experimental conditions employed in this study, an oxygen stage subsequent to an LMS treatment did not yield substantial delignification. This inefficiency could be linked to the oxidized nature of the residual lignin after an LMS. We have previously shown that the nature of the residual lignin of an LMS treated pulp is enriched with carboxylic acid groups and with quinone type structures, and is depleted of phenolic hydroxyl goups [9,16]. Hence, if an LMS treated pulp is further subjected to an oxygen delignifcation stage, then we might expect that some of the oxygen chemistry will be impeded. Presumably, the alkalinity of the oxygen system is directed towards the ionization of acid groups, the solubilization of already oxidized lignin material, and the destruction of quinone type structures. Hence, less oxygen deligmfication chemistry occurs. The same rationale could also be applied to the observed delignification response of the 0 stage subsequent to the OL treatment (i.e., OLO). Based on the experimental protocol used in this study, the delignification response of the LLE and OLE sequence was comparable to that of a 00 stage and better than that of a single 0 stage. In addition, the LE treatment responded more favorably than a single 0. Overall, the LMS delignification system exhibits an additive effect that is reflected in the percent delignification of the LE and LLE treatments. Clearly, these results highlight the efficiency of the laccase-mediator system. 10 - 60 50 The incorporation of an L treatment between a double oxygen stage was also beneficial, since the terminal viscosity was higher than that of a double oxygen treatment. Furthermore, the viscosity of an OLO treatment was comparable to a single 0 stage. In turn, this may prove to be an attractive approach in the future for obtaining the typical enhanced delignificationbenefits from a double oxygen stage without fkther loss in pulp viscosity. Nonetheless, further experimental work will be needed to support this claim. Brightness The brightness data shown in Figure 5 demonstrate that an LMS treatment leads to pulp darkening. This effect is attributed to the formation of quinone structures during an L treatment [ 161. The alkaline extraction stage subsequent to an L treatment was beneficial in regaining some of the brightness loss, obviously because of the well-known ability of NaOH to destroy quinone type structures. The combination of LMS with oxygen had less of a detrimental effect on brightness than LMS alone. Overall, the brightness results suggest that if an LMS system is to be a viable technology then the darkening effect will need to be addressed. We believe that further bleaching with peroxide could be a viable approach in dealing with this problem. However, further studies will be needed to validate this claim. 40 20 59 M 26 16 10 14 X 12 9 L BS LE LLE LO 0 00 OLE OLO 10 T-nt Figure 2. Kappa numbers of brownstock (BS) and pulps treated with 0,L, and O h . a 6 4 Viscosity Accompanying the substantial delignificationresponse of a laccase-mediator system was a high retention in pulp viscosity. The viscosity results shown in Figure 3 indicate that L,LE,and LLE treatments are much more selective than an 0 or a 00 stage. An L treatment applied after an oxygen delignification stage was more beneficial to the viscosity than when applied before, which reemphasizes the uniqueness of the enzymatic system. L LE LLE LO 0 m.nD 00 OLE OLO Figure 3. Terminal viscosity of pulps treated with 0, L, and OL. 2 b BS L IS LO UE 0 00 OLE OLO T W w I Figure 4. Brightness of brownstock (BS) and pulps treated with 0, L, and O K . CONCLUSIONS In summary, our results suggest that substantial delignification with high retention in pulp viscosity can be achieved via a laccase-violuric acid system. This study examined the delignification capabilities of an LMS system operating under extreme conditions (i.e., kappa # 73). The observed selectivity of the LMS system should provide a technology in the future to delignify kraft pulps with high yields. It is now well established that the yield benefits of stopping a kraft cook prior to reaching the residual phase can be achieved with SW kraft pulps of kappa # 40-50.Based on our studies using a kappa 75 SW haft pulp, we believe that a 50% delignification level using the lower kappa pulps (i.e. kappa # 40-50)is readily achievable with retention of pulp viscosity. Nonetheless, several research issues remain to be addressed. The loss of brightness during an LMS treatment of high-kappa pulps is a high-priority issue that will need to be examined. ACKNOWLEDGEMENTS The authors would like to thank Drs. D i m e 1 and Lucia for their guidance as well as the Institute of Paper Science and Technology and its member companies for their support for these ongoing studies. The authors would also like to express their gratitude to Potlatch Corp. Cloquet, MN for pulping the chips, and Novo Nordisk Biochem Franklinton, NC for furmshing the laccase needed for these studies. Portions of this work were used by FSC as partial Mfillment of the requirements for the Ph.D. degree at IPST. RFERENCES 1. McDONOUGH, T.J., BURTON, J.T., YETHON, A.E., “A Model for Predicting Yield in Oxygen Delignification of Softwood Kraft Pulps”, 1999 TAPPI Pulping Conference Proceedings, Orlando, FL,171-182. 2. STEFFES, F., BOKSTROM, M., NORDEN,S., “Pulp Yield Improvements Using Two-stage, Extended Oxygen Delignification”, 1998 TAPPI Proceedings. Breaking the pulp Yield Barrier Symposium, TAPPI PRESS, Atlanta, GA, 183195. 3. BOKSTROM, M., NORDEN, S., ‘Extended Oxygen Delignification”, 1998 International Pulp Bleaching Conference Proceedings, Helsinki, Finland, 23-29. 4. MAGNOTTA, V., KIRKMAN, A., JAMEEL, H., GRATZL, J., “High-Kappa-[No.] Pulping and Extended Oxygen Delignification to Increase Yield”, 1998 TAPPI Proceedings: Breaking the Pulp Yield Barrier Symposium Breaking, TAPPI PRESS, Atlanta, GA, 165-182. 5. JAMEEL, H., KIRKMAN, A., GRATZL. J., MAGNOTTA V., “High Kappa Pulping Followed by Extended Oxygen Delignification”, 1997 TAPPI Pulping Conference Proceedings, San Francisco, CA, 839. 6. PARTHASARATHY, V.R, “Is Extended Cooking Technology Necessary for the Closure of Bleach Plant? A Strategic Shift in Pulping and Bleaching”, 1997 TAPPI Pulping Conference: Biological Sciences Symposium Proceedings, San Francisco, CA, 739-757. 10. SEALEY, J.E., RUNGE, T.M., RAGAUSKAS, A.J., “Biobleaching of Kraft Pulps with Laccase and Hydroxybenzotriazole”, 1997 TAPPI Pulping Conference: Biological Science Symposium Proceedings, San Francisco, CA, 335-338. 11. POPPIUS-LEVLIN, K., WANG, W., RANUA, M., “TCF Bleaching of Laccasehiediator-Treated Kraft Pulps”, 1998 International Pulp Bleaching Conference Proceedings, Helsinki, Finland, 77-85. 12. AMANN, M., ‘The Lignozym Process -Coming Closer to the Mill”, 9” International Symposium on Wood and Pulping Chemistry Conference Proceedings, Montreal, Canada, F4-1-F45 (1997). 13.PAICE, M.G.,BOURBONNAIS, R., REID, I.D., ARCHIBALD, F.S., JURASEK, L., “Oxidative Bleaching Enzymes: A Review”, J. Pulp Paper Sci.21(8):5280-J284 (1995). 14. BALAKSHIN, M., CHEN, C-H., GRATZL, J.S., KIRKMAN, A.G., JAKOB, H., ‘Kinetics of Pulp Delignification withlaccase-Mediator System”, 5” European Workshop on Lignocellulosics and Pulp Conference Proceedings, Aveiro, Portugal, 585-588 (1998). 15. CALL, H.P., MUCKE, I., “Further Improvements ofthe Laccase-Mediator-System (LMS) for Enzymatic Delignification (Bleaching) and Results fkom Large Scale Trials”, 1995 International Non-Chlorine Bleaching Conference, Amelia Island, FL, Session 4, Paper no. 3. 16. CHAKAR, F.S., RAGAUSKAS, A.J., “ Structural Enhancement of Laccase Lignin Reactions”, 219’hNational American Chemical Society Meeting: Fundamental and Catalysis of Oxidative Delignification Processes, San Francisco, CA (March 2000). 17.0XLEY,P.W., ADGER,B.M., SASSE, M.J., FORTH, M.A., ‘W-Acetyl-N-phenylhydroxylaminevia Catalytic Transfer Hydrogenation of Nitrobenzene Using Hydrazine and Rhodium on Carbon”, Org. Synfh. 67, 187-191 (1989). 7. PRASAD, B., JAMEEL, H., MAGNOTTA, V., KIRKMAN, A., “High-Kappa Pulping and Extended Oxygen Delignification Decreases Recovery Load”, Tappi J. 77(11):135-147 (1994). 18.WORINEN, T., FAGERSTROM, P., BUCHERT, J., TENKANEN, M., TELEMAN, A., “Selective hydrolysis of hexenuronic acid groups and its application in ECF and TCF bleaching of kraftpulps”, J: Pulp Paper Science, 25(5), 155-162 (1999). 8. CHAKAR, F.S., RAGAUSKAS, A.J., NILVEBRANT, N.O., “Biobleaching of High Lignin Content Kraft Pulps via LaccaseMediator Systems”, 1998 TAPPI Pulping Conference F’roceedings, Montreal, Canada, 109-118. 19. TAPPI Test Methods 1998-1999. T 236 cm-85. TAPPI Press, Atlanta 20. TAPPI Useful Methods 1991. U246. TAPPI Press, Atlanta. 9. CHAKAR, F.S., RAGAUSKAS, A.J., ‘Fundamental Investigation of Laccase Mediator Delignification on High Lignin Content &aft p~lps”,10” International ~ymposiumon Wood and Pulping Chemistry Conference Proceedings, Yokohama, Japan, 1-566-1-571 (1999). 21. TAPPITest Methods 1998-1999. T 452 om-98. TAPPI Press, Atlanta. 22. TAPPI Test Methods 1998-1999. T230 om-94. TAPPI Press, Atlanta.